On the phenomenon of large photoluminescence red shift in GaN nanoparticles
© Slimane et al.; licensee Springer. 2013
Received: 16 July 2013
Accepted: 24 July 2013
Published: 31 July 2013
We report on the observation of broad photoluminescence wavelength tunability from n-type gallium nitride nanoparticles (GaN NPs) fabricated using the ultraviolet metal-assisted electroless etching method. Transmission and scanning electron microscopy measurements performed on the nanoparticles revealed large size dispersion ranging from 10 to 100 nm. Nanoparticles with broad tunable emission wavelength from 362 to 440 nm have been achieved by exciting the samples using the excitation power-dependent method. We attribute this large wavelength tunability to the localized potential fluctuations present within the GaN matrix and to vacancy-related surface states. Our results show that GaN NPs fabricated using this technique are promising for tunable-color-temperature white light-emitting diode applications.
KeywordsGallium nitride nanoparticles Ultraviolet electroless etching Large tunable emission Photoluminescence red shift Potential fluctuation Surface state effect
Optical properties of GaN nanostructures are of great current interest because of the potential application in solid-state lighting [1, 2]. In n-type GaN, an ultraviolet (UV) peak at approximately 3.42 eV usually dominates the photoluminescence (PL) spectrum . The blue luminescence at 2.7 to 3 eV peak energy has been extensively studied; this peak dominates due to optically active defects and impurities . Although such defects can be destructive in a device, a well-engineered inorganic nanoparticle approach can offer many advantages . Despite enormous efforts in studying the GaN defect-related emissions , there is still a research gap in explaining the origins of PL shift with optical power injection . The localized potential fluctuations within the GaN matrix introduced by the Ga vacancies and impurities are considered in explaining the PL shifts . Reshchikov et al. observed a blueshift with increasing power due to the potential fluctuation in bulk p-type GaN . On the other hand, in nanostructures having a large specific area, the surface states effect became significant in influencing the carrier recombination mechanism . However, to our knowledge, a large PL red shift with increasing excitation power was not reported and requires further investigations.
In this paper, we demonstrated the fabrication of a group III nitride-based nanoparticle (NP) using a UV-assisted electroless chemical etching method and explained the switchover in optical emission mechanism from defect-dominated to bulk-dominated PL transitions. The resultant GaN NPs are chemically stable, simple to fabricate, and easy to integrate and, most importantly, offer tunable broadband emission. We studied the emission mechanism of such novel GaN NPs, which showed controllable red shift of approximately 80 nm (approximately 600 meV) with increased optical excitation power. The tunability feature renders these nanoparticles as a good candidate for further development of tunable-color-temperature III-N-phosphor-based white light-emitting diodes (LEDs) which are essential for matching room lighting with human circadian rhythms .
The substrate used in this study consisted of a 30-μm-thick Si-doped GaN epitaxy grown on c-plane (0001) sapphire (α-Al2O3) substrate with a measured resistivity of less than 0.03 Ω cm. The estimated dislocation density and measured carrier concentration of the film are 1 × 108 cm−2 and 2 × 1018 cm−3, respectively. Prior to wet etching in a HF/CH3OH/H2O2 (2:1:2) solution under UV illumination, 10-nm thin strips of platinum (Pt) were sputtered onto the GaN samples at one end of the surface to complete the loop for electron–hole exchange between semiconductor and electrolyte . The resultant nanostructure layers were later transferred onto a Si wafer at subsequent room temperature and 77 K for PL measurements using Jobin Yvon’s LabRAM ARAMIS microphotoluminescence (μPL) spectroscopy system (HORIBA, Ltd., Minami-ku, Kyoto, Japan). The optical excitation was produced using a helium-cadmium (HeCd) laser emitting at 325 nm with a <10-μm spot size. The scanning and transmission electron microscopy (SEM and TEM) investigations were performed using FEI Quanta 600 and FEI Titan G2 80–300 electron microscopes (FEI Co., Hillsboro, OR, USA), respectively.
Results and discussion
The μPL spectrum of the GaN NPs presents approximately 110-meV red shift that could be attributed to the relaxation of the compressive strain , but foremost, we observe a relatively strong/prominent increase of the DAP and Iox peak intensities. In the n-type GaN DAP transitions, these acceptor-like sites have been reported by a number of authors to originate from Ga vacancies (VGa) [14, 15]. The GaN NPs underwent chemical etching, thus resulting in an increase of oxygen and vacancy sites at the surface due to the competition between the formation and dissolution of Ga x O y (Figure 1c). This explains the increase in the emission intensity of DAP peaks.
The power-dependent PL measurement was performed on the NPs. Figure 2b shows a typical room temperature μPL emission spectrum of the as-grown GaN excited at 0.08 kW/cm2 together with the excitation power-dependent μPL emission spectrum of the GaN NPs. Compared to the 77 K PL, we observe in the room temperature PL of the as-grown sample a quenching of D0X peak while the FX emission became dominant at 3.42 eV (approximately 362 nm). The broadening in the lower photon energy due to the oxygen impurity is still observable whereas the DAP peak disappeared. Most importantly, room temperature PL of GaN NPs excited at 0.08 kW/cm2 exhibits a luminescence peak centered at 3.353 eV (369 nm) which is red-shifted by 69 meV compared to the as-grown sample. As the excitation power increases from 0.08 to 8 kW/cm2, we observe an approximate linear decrease of the peak PL photon energy with a total span of 530 meV (Figure 2c). We investigated several spots in the as-grown GaN bulk epitaxy, but no shift with increasing excitation power was observed. Besides the red shift, the measured FWHM shows a direct dependence over the excitation power as it increases from 120 meV (approximately 13 nm) at 0.08 kW/cm2 to 263 meV (approximately 40 nm) at 8 kW/cm2 (Figure 2c). Such a wide FWHM is twice as large as the measured FWHM of the peak from the as-grown GaN bulk epitaxy where the linewidth broadening at the same power density is 42 meV (approximately 4.5 nm). This FWHM widening indicates a contribution of inhomogeneous broadening in the clusters of NPs.
In bandgap renormalization, the formation of ionization and electron hole plasma leads to the bandgap narrowing . Calculations specific to our material and experimental conditions, based on the empirical relation ΔE = kn 1/3 reported by Lee et al. , where k is the bandgap renormalization coefficient (k ~ 10−8 eV cm), E is the bandgap energy, and n is the carrier density, predict a bandgap narrowing in the order of 20 meV. This prediction is inconsistent with our experimental measurements, specifically considering the large red shift measured, so bandgap renormalization can be safely neglected as a plausible cause.
Due to the Coulomb interaction, transitions related to DAP blueshift with increasing excitation intensity. In fact, the photon energy (hυ) is inversely proportional to the distance, r, between neutral acceptors and donors, i.e., hυ ∝ 1 / r. With increasing excitation power, the distance decreases, and as a consequence, the photon energy blueshifts by a few millielectron volt . Conversely, in our case, a significant red shift is observed, and hence, we might ignore the blueshift caused by the Coulomb interaction in these transitions.
The GaN used in this study is n-doped and has a carrier density of 2 × 1018 cm−3; thus, the red shift might be due to the presence of an impurity band generated from doping concentrations .
The potential fluctuations model, on the other hand, explains this large red shift in the PL with increasing excitation power. It is known that the crystalline orientation distortions cause effective bandgap dispersion and thus creates lateral potential fluctuations. Vacancies, impurities, dangling bonds, and strain and structural defects all introduce these fluctuations [18, 19]. In our case, the material underwent chemical electroless etching from which a different structural shape and strain in the NPs arises . This coalescence of the NPs induces the formation of boundary dislocations, and additionally, the preferential etching increases the impurity and vacancy defect concentration .
Furthermore, due to the extremely high surface-to-volume ratio of the produced NPs paired with localized potential fluctuation, surface states cannot be neglected. The n-type GaN NPs have surface defects; thus, we have band bending in these regions (Figure 4). The creation of surface depletion will change the emission in the GaN NPs. The calculated width of the depletion region in our case is d ~ 24 nm, given by  where ϵGaN is the static dielectric constant of GaN, Vbi the potential at the boundary, q the electronic charge, and Nd the donor density. The NP with a width W < 2d will be totally depleted. VGa centers acting like acceptor sites will be depleted from holes, and FX transitions will dominate. If W > 2d, both depletion region and non-depletion region can exist. Furthermore, by increasing the excitation power or temperature, the depletion region decreases and the Fermi level increases. Thus, holes populate the acceptor-like sites in the depletion region and electrons populate the donor states; therefore, we have an increase of DAP and donor-like oxygen states and acceptor-like VGa states. This leads to the visible blue emission at higher excitation power. In Figure 4c, the depletion region is a collective representation of trap states due to sharp edges within a NP and across different NPs with size inhomogeneity evident in Figure 1. The sharp edges and/or smaller NP sizes enhance oxidation and therefore increase the density of states and carrier capture cross section of carrier traps, i.e., localized states. In addition, the smaller the NP, the higher the conduction band minima of the local potential fluctuation. The LO phonon enhancement is due to indirect transition from the silicon donor states to the valence band maxima of the local potential fluctuation, which confirms the PL peak broadening.
The emission yield, tenability, and FWHM of our NPs can be modified by controlling the NP size and inhomogeneity. With further process optimization and postprocessing treatments through, for example, annealing and surface passivation, the quality of the quantum yield of the oxide-encapsulated GaN NPs can be improved.
In summary, GaN nanoparticles with size dispersion between 10 and 100 nm have been fabricated using the UV metal-assisted electroless etching method. A large emission wavelength tunability of approximately 530 meV has been observed from the nanoparticles. We demonstrated that the localized potential fluctuation and surface state effects are responsible for such shift. These fabricated oxide-encapsulated GaN nanoparticles can be used as phosphor for tunable-color-temperature white LED application.
The authors would like to thank the Advanced Nanofabrication, Imaging and Characterization (ANIC) Laboratory, KAUST for the use of their facilities.
- Nguyen HPT, Zhang S, Cui K, Han X, Fathololoumi S, Couillard M, Botton GA, Mi Z: P-type modulation doped InGaN/GaN dot-in-a-wire white-light-emitting diodes monolithically grown on Si(111). Nano Letters 2011, 11: 1919–1924. 10.1021/nl104536xView ArticleGoogle Scholar
- Johnson JC, Choi HJ, Knutsen KP, Schaller RD, Yang P, Saykally RJ: Single gallium nitride nanowire lasers. Nat Mater 2002, 1: 106–110. 10.1038/nmat728View ArticleGoogle Scholar
- Song KM, Kim H: Optical properties of undoped a -plane GaN grown with different initial growth pressures. Jpn J Appl Phys 2012, 51: 092101.View ArticleGoogle Scholar
- Reshchikov MA, Morkoç H: Luminescence properties of defects in GaN. J Appl Phys 2005, 97: 061301–061395. 10.1063/1.1868059View ArticleGoogle Scholar
- Slimane AB, Najar A, Ng TK, Ooi BS: Thermal annealing induced relaxation of compressive strain in porous GaN structures. In Proceedings of the 25th IEEE Photonics Conference: 23–27 September 2012; Burlingame. California: IEEE; 2012:921–922.View ArticleGoogle Scholar
- Wang H, Ji Z, Qu S, Wang G, Jiang Y, Liu B, Xu X, Mino H: Influence of excitation power and temperature on photoluminescence in InGaN/GaN multiple quantum wells. Optics Express 2012, 20: 3932–3940. 10.1364/OE.20.003932View ArticleGoogle Scholar
- Cho YH, Gainer GH, Fischer AJ, Song JJ, Keller S, Mishra UK, DenBaars SP: “S-shaped” temperature-dependent emission shift and carrier dynamics in InGaN/GaN multiple quantum wells. Appl Phys Lett 1998, 73: 1370–1372. 10.1063/1.122164View ArticleGoogle Scholar
- Reshchikov MA, Xie J, He L, Gu X, Moon YT, Fu Y, Morkoç H: Effect of potential fluctuations on photoluminescence in Mg-doped GaN. Phys Stat Sol (C) 2005, 2: 2761–2764. 10.1002/pssc.200461370View ArticleGoogle Scholar
- Liao ZM, Zhang HZ, Zhou YB, Xu J, Zhang JM, Yu DP: Surface effects on photoluminescence of single ZnO nanowires. Phys Lett A 2008, 372: 4505–4509. 10.1016/j.physleta.2008.04.013View ArticleGoogle Scholar
- Kim JK, Schubert EF: Transcending the replacement paradigm of a solid-state lighting. Opt Express 2008, 16: 21835–21842. 10.1364/OE.16.021835View ArticleGoogle Scholar
- Bardwell JA, Webb JB, Tang H, Fraser J, Moisa S: Ultraviolet photo enhanced wet etching of GaN in K2S2O8 solution. J Appl Phys 2001, 89: 4142–4149. 10.1063/1.1352684View ArticleGoogle Scholar
- Chung BC, Gershenzon M: The influence of oxygen on the electrical and optical properties of GaN crystals grown by metalorganic vapor phase epitaxy. J Appl Phys 1992, 72: 651–659. 10.1063/1.351848View ArticleGoogle Scholar
- Fischer S, Wetzel C, Hansen WL, Bourret-Courchesne ED, Meyer BK, Haller EE: Properties of GaN grown at high rates on sapphire and on 6H-SiC. Appl Phys Lett 1996, 69: 2716–2718. 10.1063/1.117688View ArticleGoogle Scholar
- Reshchikov MA, Shahedipour F, Korotkov RY, Wessels BW, Ulmer MP: Photoluminescence band near 2.9 eV in undoped GaN epitaxial layers. J Appl Phys 2000, 87: 3351–3354. 10.1063/1.372348View ArticleGoogle Scholar
- Boguslawski P, Briggs EL, Bernholc J: Native defects in gallium nitride. Phys Rev B 1995, 51: 17255–17258. 10.1103/PhysRevB.51.17255View ArticleGoogle Scholar
- Lee IH, Lee JJ, Kung P, Sanchez FJ, Razeghi M: Band-gap narrowing and potential fluctuation in Si-doped GaN. Appl Phys Lett 1999, 74: 102–104. 10.1063/1.122964View ArticleGoogle Scholar
- Kaufmann U, Kunzer M, Maier M, Obloh H, Ramakrishnan A, Santic B, Schlotter P: Nature of the 2.8 eV photoluminescence band in Mg doped GaN. Appl Phys Lett 1998, 72: 1326–1328. 10.1063/1.120983View ArticleGoogle Scholar
- Oh E, Park H, Park Y: Influence of potential fluctuation on optical and electrical properties in GaN. Appl Phys Lett 1998, 72: 1848–1850. 10.1063/1.121203View ArticleGoogle Scholar
- Reshchikov MA, Yi GC, Wessels BW: Behavior of 2.8- and 3.2-eV photoluminescence bands in Mg-doped GaN at different temperatures and excitation densities. Physical Review B 1999, 59: 13176. 10.1103/PhysRevB.59.13176View ArticleGoogle Scholar
- Zhuang D, Edgar JH: Wet etching of GaN, AlN, and SiC: a review. Mater Sci Eng R 2005, 48: 1–46. 10.1016/j.mser.2004.11.002View ArticleGoogle Scholar
- DeLong MC, Taylor PC, Olson JM: Excitation intensity dependence of photoluminescence in Ga0.52In0.48P. Appl Phys Lett 1990, 57: 620–622. 10.1063/1.103615View ArticleGoogle Scholar
- Vanheusden K, Warren WL, Seager CH, Tallant DR, Voigt JA, Gnade BE: Mechanisms behind green photoluminescence in ZnO phosphor powders. J Appl Phys 1996, 79: 7983–7990. 10.1063/1.362349View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.